EFFECT OF PRIOR MICROSTRUCTURE ON AUSTENITE DECOMPOSITION ... effect of prior microstructure on...
Embed Size (px)
Transcript of EFFECT OF PRIOR MICROSTRUCTURE ON AUSTENITE DECOMPOSITION ... effect of prior microstructure on...
EFFECT OF PRIOR MICROSTRUCTURE
ON AUSTENITE DECOMPOSITION AND
R. Ramanathan and R. P. Foley
MMAE Department Illinois Institute of Technology
10 West 32nd Street Chicago, IL 60616-3793
312-567-3052p / 312-567-8875f / firstname.lastname@example.org http://mmae.iit.edu/~foleyweb/
Steel components are heat treated in order to obtain desired microstructure and properties. However, such heat treatments often also impart unwanted and often unpredictable dimensional changes . In the present work, Jominy bars are used to characterize the pattern of the dimension change versus distance from the quenched end and versus initial starting microstructure. The behavior of nine different kinds of steels is investigated.
Size distortion is characterized as part growth or shrinkage. It is generally attributed to the volume differences between the various phases developed in the microstructure of a steel component during heat treatment. The martensitic microstructure of a particular steel, for example, has a slightly higher specific volume (lower density) than the same steel with a ferrite- pearlite microstructure. The specific volume differences between the various phases generally increase with the alloy carbon content. Shape distortion is associated with mechanisms that produce microstructure variations within the component. These microstructure differences may be inherited from casting and hot working or may result from an uneven thermal cycle.
Experiments with carburized and oil-quenched annular discs produced from different steels have shown that the dimension changes could be related to steel hardenability. The dimensional changes were found to be a function of steel hardenability only as long as the alloy composition was insufficient to through harden the part so to produce a 100% martensitic core. Disks made from alloy compositions with sufficient hardenability all showed similar distortion behavior . In general a majority of the variability in distortion behavior can be related to the variability in the transformation behavior of the steel used to make the part and the variability in the thermal cycle used to process the part. Sensitivity to distortion variability seems to be related to the consistency with which a particular steels austenite decomposes to produce a specific microstructure distribution within a part.
Factor influencing the austenite decomposition include the alloy chemistry, the austenite grain size, and the local cooling path. As a result, similar cooling paths lead to similar distortion patterns and the decomposition of austenite in similar fashion leads to similar distortion pattern. Fukuzumi and Yoshimura showed that small variations in aluminum content (Al/N ratio) in 8620 and 4120 low-alloy steel produces pronounced distortion pattern differences in Navy C-rings that may be related to differences in the CCT (continuous cooling transformation) behavior of the steels .
Microsegregation in large-tonnage low-cost steel products is unavoidable. Alloy solidification behavior during casting and the subsequent hot working process produces elemental banding and possibly microstructure banding as well. Elemental banding results from interdendritic segregation and is related to the difference between the alloy liquidus and solidus temperatures. Microstructure banding results from carbon diffusion to regions of the microstructure where elemental banding produces a high local affinity for carbon and the subsequent decomposition of these regions into various austenite decomposition products. Microstructure variability associated with microsegregation of alloying elements has been postulated as being one of the likely important contributors to hardness and geometry variations of forged and heat-treated
components . Such segregation produces a position sensitive alloy composition and transformation behavior. These effects may lead to complicated distortion and residual stress patterns. In high-carbide tool steels, for example, size change directionality due to heat treatment has been attributed to microstructure changes associate with the redistribution of carbides from a state of preferential alignment to one of more random alignment .
Transformation of austenite is routinely characterized by the Jominy end-quench test. In this work, the end-quench test is used to characterize the transformation and distortion behavior of nine different types of steels. Hardness profiles, the common result of such test, are combined with measurements of diameter change to characterize the relationship between alloy chemistry and prior microstructure on the hardenability and distortion pattern developed in the steels.
Figure 1 shows a conventional flat machined in the Jominy by removing 0.015in layer along its length. A diameter variation along the length can be seen as an hourglass shape on a close look at the ground strip, the difference in the diameter of the bar at various distances from the quenched end results from the decomposition of austenite .
Figure 1 – Hourglass distortion patterns can be seen near the quenched end in flat ground in the Jominy bars due to diameter variation along the length.
Table 1 shows the chemical compositions of the nine steels used in this investigation. Some of the steels were selected such that they fairly represent the steels used in the forging industry and the others were selected because they may offer insight to the mechanism responsible for the distortion pattern. The steel set consisted of machinable grade 12L14 and 1117, plain low carbon 1018 steel, carburizing grade 8620 alloy steel, low hardenable, medium carbon 1045 steel, high hardenable, medium carbon 4140 steel, W1 and O1 tool steel and 304 austenitic stainless steel. The steels were purchased as bar stocks of 1.5in diameter. The chemical compositions of the steels were taken from literature.
TABLE 1 - Composition range of steel used in the present investigation (wt-pct).
Figure 2 schematically shows the experimental procedures used in this work. Three 7in long sections were cut from the bar stock of the nine different steels and each of these three sections was individually heated to austenitizing temperature (900 +/- 5°C is maintained for all the bars) and held at this temperature for an hour in a laboratory box furnace. Following this, the bars were cooled in still air (air-cooled), in the furnace (furnace-cooled) or in oil (oil-quenched) to produce three different starting microstructures. Twenty-seven Jominy bars were obtained from nine different steels and three different initial microstructures thus produced. Jominy bars were machined in a HAAS SL – 20 CNC lathe. The sections from the end piece of the heat-treated bars were used to obtain metallographic samples for characterizing the initial microstructure in the longitudinal direction and the hardness profile across the diametric cross section.
The exact geometry of the Jominy bars were slightly different from the standard Jominy bars geometry in that each had a flat-machined perpendicular to the axis in the head and four grooves of specific dimension from specific distance from the end along the circumference of the Jominy bar. The purpose of the flat was to ensure similar positioning of the Jominy bars in the fixture
Figure 2 – Schematic overview of experimental test procedure
during the distortion measurements and the purpose of the grooves were to align the distortion data points before and after end quenching.
Distortion of the bars was characterized as change in bar diameter versus distance from quenched end. The diameter change was determined as the difference between the profile diameters measured before and after end quenching. The scanning of the Jominy bar was carried out in a Mitutoyo CBH-400 Contracer, this tracer was able to record vertical distance to 0.000008in and horizontal distance to 0.00001in. The Jominy bar was clamped in a jaw attached to an indexing head after ensuring that the flat in the jominy bar is parallel to the surface table using a dial gage with 0.0005in least count. The scanning was carried out along the length of the bar for every 30deg. The bar was then end quenched in confirmation with ASTM standard 255 . The bars were heated to austenitizing temperature for 45min (900 +/- 5°C maintained for all bars) in a laboratory box furnace in a close fitting, closed-end stainless steel sleeve with cast iron pieces at the closed end to prevent oxidation. Since the head of the bar was not protected from oxidation by covering with a fixture the scale formed in the head was removed by a very mild sand blasting. The end-quenched bar was then scanned again in the Mitutoyo CBH-400 Contracer following the same procedure as before. The hardness measurement was also carried in confirmation with the ASTM standard 255 with flats ground to 0.015in and the hardness reported as the average of the hardness value from both the flats .
RESULTS AND DISCUSSION
Figures 3 to 11 show the light optical micrographs of various steels along longitudinal direction of the bar under various heat treatment conditions. The microstructure of each steels in 100X and 400X original magnification are shown adjacently with furnace cooled (FC) on top, air cooled (AC) in the middle and oil quenched (OQ) at the bottom of the page for each steels.
In general, the microstructure refines as the cooling rate progress